Fluid-crystal coexistence for proteins and inorganic nanocolloids:
Dependence on ionic strength
Peter Prinsen and Theo Odijka兲
Complex Fluids Theory, Faculty of Applied Sciences, Delft University of Technology, 2628 BC Delft, The Netherlands
共Received 11 April 2006; accepted 19 July 2006; published online 18 August 2006兲
We investigate theoretically the fluid-crystal coexistence of solutions of globular charged nanoparticles such as proteins and inorganic colloids. The thermodynamic properties of the fluid phase are computed via the optimized Baxter model P. Prinsen and T. Odijk关J. Chem. Phys. 121, 6525 共2004兲兴. This is done specifically for lysozyme and silicotungstates for which the bare adhesion parameters are evaluated via the experimental second virial coefficients. The electrostatic free energy of the crystal is approximated by supposing the cavities in the interstitial phase between the particles are spherical in form. In the salt-free case a Poisson-Boltzmann equation is solved to calculate the effective charge on a particle and a Donnan approximation is used to derive the chemical potential and osmotic pressure in the presence of salt. The coexistence data of lysozyme and silicotungstates are analyzed within this scheme, especially with regard to the ionic-strength dependence of the chemical potentials. The latter agree within the two phases provided some upward adjustment of the effective charge is allowed for. © 2006 American Institute of Physics. 关DOI:10.1063/1.2336423兴
One current view of protein crystallization centers on the second virial coefficient B2 being a relevant quantity deter-mining the onset of crystallization.1–4There exists a crystal-lization slot of negative B2 values which expresses a neces-sary range of solution conditions for adequate crystals to grow. A negative value of B2 implies a Baxter stickiness parameter as it is conventionally defined via B2only and we here denote by 0. Thus, in a similar vein, there have been attempts to correlate0with the solubility of nanoparticles in explaining fluid-crystal coexistence curves.5,6
The free energy of a suspension of particles cannot, of course, depend on B2alone. In a recent paper7we introduced a new analytical theory for protein solutions in which the real fluid is replaced by a suspension of spheres with an appropriately chosen adhesion of the Baxter type. The sticki-ness parameter is computed by a variational principle for the free energy instead of via B2. In our optimized Baxter model, is not at all identical to0; depends not only on the ionic strength but also on the protein concentration. In Ref.5, Rosenbaum et al. plotted0logarithmically as a func-tion of the nanoparticle concentrafunc-tion which effectively coarse-grains the experimental data they show. If we zoom in on their curve, there is a lot of fine detail which we here argue to be related to the fact, in part, that is a better similarity parameter. In particular, we seek to understand the ionic-strength dependence of the fluid-crystal coexistence curves by going beyond theory based solely on0.
We have recently tested the optimized Baxter model on a
system of spheres interacting via an attractive Yukawa poten-tial analyzed by computer simulations.8 The stickiness pa-rameter, evaluated by optimizing the free energy, is indeed a useful similarity variable for gaining insight into the pres-sures and chemical potentials from simulations of the fluid phase. The magnitudes of these quantities are also well pre-dicted by the optimized Baxter model. However, is not a correct similarity variable to describe fluid-crystal coexist-ence as we show in Appendix A, in view of the fact that the weighting of configurations is different in the respective phases.
Here, we will not focus on the variable and the fluid phase but rather on the coexistence itself. The systems we study are assumed to have a short enough range so that the coexistence between two fluid phases is apparently circum-vented. An a priori theory is problematic because we would need a quantitative theory of the crystal phase in terms of postulated attractive forces which are currently unknown. Theoretical efforts exist in the literature9–11at the expense of introducing unknown parameters which we want to avoid here. We do not present conventional phase diagrams be-cause we do not know the right thermodynamic variable to plot to get a universal diagram of states. The variableitself is not useful as we show in Appendix A.
In practice, it may be very difficult to achieve ideal ther-modynamic equilibrium between the liquid phase and some crystalline state. Equilibrium may not have been reached, the crystal could be heterogeneous and the formation of aggre-gates could complicate the attainment of equilibrium 共see, for instance, the discussion by Cacioppo and Pusey on lysozyme12兲. Nevertheless, it may still be useful to assume that equilibrium is ideally attained provided our goal is suf-ficiently modest. The balance of chemical potentials has been
a兲Author to whom correspondence should be addressed. Present address:
P.O. Box 11036, 2301 EA Leiden, The Netherlands. Electronic mail: email@example.com
used before to acquire information about the crystal from the solubility in the fluid phase.3Our concern here will be to try to gain insight into the ionic-strength dependence of the ther-modynamic properties of the crystal. We may argue that this dependence could be approximated by a Donnan equilibrium so it would not be very sensitive to the precise crystal habit adopted. We therefore compute the protein chemical poten-tial and osmotic pressure of the coexisting liquid phase at the experimentally determined solubility with the help of the op-timized Baxter model. We then investigate whether their de-pendence on the electrolyte concentration agrees with that predicted by a simple crystal model. The theory is applied to a protein 共lysozyme兲 and an inorganic nanocolloid 关silico-tungstate共STA兲兴.
II. OPTIMIZED BAXTER MODEL
We first discuss how we obtain the bare adhesion param-eters via the second virial coefficient, and then summarize the optimized Baxter model,7 which is an appropriate liquid state theory provided we use the right stickiness parameter as emphasized in the Introduction. We consider a system of charged nanometer-sized particles共e.g., proteins or nanocol-loids兲 in water with added monovalent salt of ionic strength
I. We suppose the particles are spherical with radius a. The
charge is distributed uniformly on the particle’s surface. For convenience, all distances in this section will be scaled by the radius a and all energies by kBT, where kBis Boltzmann’s constant and T is the temperature. Because monovalent ions 共counterions and salt ions兲 are present in solution, the Cou-lomb repulsion between the particles will be screened and it is here given by a far-field Debye-Hückel potential.7 The effective number Zeffof charges on the sphere 共taken to be positive兲 will here be computed in the Poisson-Boltzmann approximation. We let the attraction between two particles be of range much shorter than their radius, and we model it by a potential well of depth UA and width ␦Ⰶ1. Actually, the attractive interactions are, of course, much more complicated than this simple form. Dispersion forces, in particular, have been reinvestigated for small particles recently13,14 although the continuum approximation certainly becomes rather poor at the nanolevel dealt with here. Also, arbitrary cutoffs need to be introduced;7 it turns out that a simple well is quite adequate to describe the experimental data on B2共see Sec. III below兲. The total interaction U共x兲 between two particles whose centers of mass are separated by an actual distance r is thus of the form
冦⬁, 0艋 x 艋 2 UDH共x兲 − UA, 2艋 x ⬍ 2 +␦ UDH共x兲, x艌 2 +␦,
冧x⬅ r a, 共1兲
with Debye-Hückel interaction
UDH共x兲 = 2
x . 共2兲
Here,⬅共Q/2a兲共Zeff/共1+兲兲2and⬅a, which are given in terms of the Debye length −1 defined by2= 8QI and
the Bjerrum length Q = q2/⑀kBT, which equals 0.71 nm in water at 298 K 共⑀ is the permittivity of water and q is the elementary charge兲; = 3.28a
冑I, if the radius a is given in
nanometers and the ionic strength I in M. We suppose 1-1 electrolyte has been added in excess so I is the concentration of added salt. We have derived the effective charge qZeffin the Poisson-Boltzmann approximation7
Zeff= Z − 2 6
冉Z 1 +
冊3 e3E1共3兲. 共3兲
Here E1共x兲 is the exponential integral defined by E1共x兲 =兰x⬁dtt−1e−tand qZ is the actual charge per particle. Equation 共3兲 is numerically consistent with a different form recently proposed by Aubouy et al.15 which is also valid at large values of Z.
We suppose that the bare charge on the particles as a function of the ionic strength is known from experiment, so the only unknown parameters are UAand␦which are chosen to be independent of I. The latter are determined by fitting preferably complete experimental data of the second virial coefficient B2as a function of the ionic strength I at constant pH to B2computed numerically with the help of the expres-sion
x2dx共1 − e−U共x兲兲 共4兲
using Eq.共1兲. We have previously done this for a wide vari-ety of B2data on lysozyme at two values of the pH 共4.5 and 7.5兲 and we were able to obtain very good fits7共see, e.g., Fig. 1 which is discussed in Sec. III B兲.
It is important to stress that though there are two adjust-able parameters␦ and UA, the actual fit in practice depends FIG. 1. The second virial coefficient of lysozyme as a function of the ionic strength. The second virial coefficient is scaled by the hard sphere value
B2HS. The data are taken from a variety of experiments; see Ref.7for more details. The added salt is NaCl. The solid line is a fit to the data with UA
almost solely on adjusting the single combination ␦exp UA. This is because a convenient analytical approximation of the second virial turns out to have the form7
B2 B2HS⯝ 1 + 3 2− 3 2e −␦eUA , 共5兲
and is able to describe the experimental data on lysozyme quite well with an appropriate value of␦exp UA. Here, B2HS is the second virial coefficient pertaining to hard spheres. The strong correlation of adjustable parameters is not un-usual for it is well known in the theory of gases when one attempts to fit the temperature dependence of the second virial coefficient in terms of a Lennard-Jones interaction, for instance.16 We note that Eq. 共5兲 disagrees starkly with an approximation put forward earlier,17both with regard to the pure electrostatic and the adhesive contributions. In particu-lar, the third, i.e., adhesion term in Eq.共5兲is not at all inde-pendent of the ionic strength but rather diminishes fast as the electrolyte concentration is lowered. Furthermore, the pure electrostatic term cannot be derived from a Donnan equilib-rium as we point out in Sec. IV.
At high salt concentrations, the parameter becomes small owing to screening so B2becomes lower than the hard sphere value, as can be seen from Eq.共5兲. Nevertheless, the electrostatic repulsion still exerts itself, so an effective adhe-sion parameter we may wish to introduce would be smaller than the bare value. We therefore adopt a similar strategy to the liquid state at finite concentrations by first introducing a suitable reference state amenable to analytical computation.7 This is a solution of hard spheres whose radius is still a but with a Baxter adhesion potential whose strength is defined by a suitable stickiness parameter. The statistical properties of this suspension as a function of the volume fraction of spheres共=4a3/ 3 times number density兲 may be solved in the Percus-Yevick approximation.18 The parameter is ad-justable and is computed via a variational principle for the free energy. The latter may be written as a functional expan-sion in terms of the so-called blip function which is the dif-ference in Mayer functions of the respective interactions关Eq.
共1兲 and the Baxter interaction兴.7,19
We set the first-order de-viation from the free energy pertaining to the reference state equal to zero. This determineswhich depends not only on the well parameters ␦ and UA and electrostatic variables and but also on the volume fraction of nanospheres. It is given by7 1 = 3⑀关共e UA e−关/共1+⑀/2兲兴e−⑀− 1兲共1 + 共1 + H兲⑀兲 +共eUAe−− 1兲兴, 共6兲 where ⑀=␦− K−1关共1 +␦H兲P1+ HP2兴, 共7兲 P1= 8 2共1 +␦兲M + 16
冉M 1 + M
冊, 共8兲 P2= 8 3共2 +␦兲M + 16 2ln共1 + M兲, 共9兲 M⬅e−␦/4, 共10兲 K = 2共eUAe−关/共1+␦/2兲兴e−␦− 1兲共1 + 共1 + H兲␦兲 + 2共eUAe−关/共1+⑀/2兲兴e−⑀− 1兲共1 + 共1 + H兲⑀兲, 共11兲 H = 2共1 −兲
冉共1 −兲 12 2−1 + 11 12 + 1 + 5 1 − − 9共1 +兲 2共1 −兲2 1
冊共12兲 and is given by = 1 +/2 共1 −兲2 1 − 1 −+ 12. 共13兲
Note that is readily obtained by iteration. One starts with initial values for and ⑀ and then calculates , H, and K1 from Eqs. 共11兲–共13兲. Then, a new value of ⑀ at fixed H is computed iteratively with the help of Eqs.共7兲and共11兲. Next, a new value of is given by Eq. 共6兲 and then the cycle is repeated until the variables become stationary.
Having obtained the effective adhesion parameter, we simply calculate thermodynamic properties of the reference state within the Percus-Yevick approximation. The free en-ergy of the actual system does deviate slightly from that of the reference state but we have shown that the deviations are very small.7To compute the osmotic pressure⌸ we use the result from the compressibility route18 which appears to be more in line with simulations,20
⌸v0 kBT =共1 ++ 2兲 共1 −兲3 − 2共1 +/2兲 共1 −兲2 + 3 36 3. 共14兲
When the roots of Eq.共13兲are complex, the pressure cannot be determined for the physical realization of the liquid state breaks down, at least with the Percus-Yevick approximation. The chemical potential of the spherical particles is deter-mined by using the pressure from Eq. 共14兲 and the Gibbs-Duhem equation at constant temperature,21
−0 kBT = ln 1 −+ 3共4 −兲 2共1 −兲2 + ⌸v0 kBT + J. 共15兲 Here, J =3 2 22−3共1 + 4兲 共1 −兲 + 6共2 +兲 共1 −兲2 − 18 1 − − 6共−c兲 2 c共1 − 6c兲 ln
冏共1 −兲 −c −1 −1− c −1
冏+6c共18c− 1兲 2 1 − 6c ln
冏共1 −兲 − 18c −1− 18 c
冏共16兲 is the contribution to the chemical potential that vanishes in the hard-sphere limit共→⬁兲 and
0 kBT = ln 1 v0
冊3/2 , 共17兲
den-sities where there is no real solution of, is given by c=
6 . 共18兲
III. SOLUBILITY CURVES: CHEMICAL POTENTIAL
OF THE FLUID PHASES A. Method
Since we suppose the crystal is in thermodynamic equi-librium with the fluid, the protein chemical potentials as well as the osmotic pressures in both phases are uniform. The chemical potentials of the counter- and coions must also be uniform but we will address this issue later within a Donnan equilibrium. Solubility data from experiment represent the particle concentration in the fluid phase as a function of the
pH and the salt concentration. Thus we compute the
chemi-cal potential and the osmotic pressure of the solution with the help of the optimized Baxter model of the previous sec-tion. We have done this in two cases of nanoparticles where we have sufficient experimental data on the second virial coefficient to evaluate the well parameters UA and ␦ with sufficient accuracy.
The protein hen-egg-white lysozyme has been well char-acterized in aqueous solutions of simple electrolytes. We here choose the effective radius a such that the volume of the model sphere is equal to the volume of a lysozyme molecule in the tetragonal crystal state. The latter is determined from the water content of the tetragonal crystal 共0.335 mass fraction22兲, the crystal volume per protein molecule 共29.6 nm3, based on the dimensions 7.91⫻7.91⫻3.79 nm3 of the unit cell containing eight protein molecules23兲, the density of the crystal关1.242⫻103kg m−3共Ref.22兲兴, and the
density of water 共0.998⫻103 kg m−3兲. Thus we have a
= 1.6 nm and note that this is 0.1 nm less than the value of 1.7 nm we used previously,7which was based on approxima-tion of the protein by an ellipsoid of dimensions 4.5⫻3.0 ⫻3.0 nm.24
For the sake of consistency we here use the single value a = 1.6 nm in computations pertaining to both phases.
The experimental data for the second virial coefficient of lysozyme have been discussed by us at length previously7 and are presented in Fig. 1. For details on determining the parameters UAand␦ of the attractive potential we also refer to Ref.7. Since we are using a smaller effective radius here, we deduce the values UA= 2.90 and ␦= 0.183 which are somewhat different from those derived earlier.7The values of the bare charge qZ of a lysozyme molecule as a function of the ionic strength are the same as those used in Ref.7, i.e., they are determined by interpolation from hydrogen-ion ti-tration data in KCl.25 We assume that KCl and NaCl 共see below兲 behave identically in an electrostatic sense. The ef-fective charge does differ slightly because it is a function of
a 关see Eq. 共3兲兴. We again use the lowered effective charge Z
¯ =Zeff− 1 instead of the effective charge Zeffin order to fit B2 accurately at lower ionic strengths when it is dominated by electrostatics. We set UAand␦ to be independent of the pH. Accurate data on the solubility S as a function of the NaCl concentration have been obtained by Cacioppo and Pusey12using column beds of tetragonal microcrystallites of lysozyme in a range of pH and temperatures. We here em-ploy their data at 298 K and at three representative values of the pH共see TableI兲 The ionic strength I in M is determined
from the ionic strength in % w / v by the relation I共M兲 = 0.06+ 0.171 I共% w/v兲. Here, the value 0.06 accounts for the effective ionic strength of the 0.1M sodium acetate buffer used and 0.171= 10/ MNaCl where MNaCl= 58.44 g mol−1 is the molar mass of NaCl. The dimensionless parameter is then given by = 5.25
冑I, where I is given in Mi and = 0.222共Z¯/共1+兲兲2.
The volume fraction of protein in the liquid phase is TABLE I. The charge Z of hen-egg-white lysozyme共from Ref.25兲, the effective charge Zeff共from Eq.共3兲兲, the lowered effective charge Z¯=Zeff− 1, the
dimensionless interaction parameters,, and, the solubility of lysozyme S, the volume fraction, the dimensionless chemical potential共−0兲/kBT, and
the dimensionless pressure⌸v0/ kbT as a function of the ionic strength I in the fluid phase.has been calculated using the lowered effective charge Z¯ .
given by= SNAv0/ M, where NA is Avogadro’s number,v0 = 4a3/ 3 is the volume of a lysozyme molecule, and M = 14.3⫻103g mol−1 共Ref. 26兲 is the molar mass of lysozyme. The parameterdescribing the effective adhesion is determined as described in Sec. II 关see Eqs. 共6兲–共13兲兴, using the values UA= 2.90 and ␦= 0.183. Then, the dimen-sionless chemical potential共−0兲/kBT and the dimension-less osmotic pressure ⌸v0/ kBT are determined from Eqs. 共15兲and共14兲, respectively共see TableI兲. Figure2shows the chemical potential as a function of the ionic strength I at three different values of the pH. Figure3shows the osmotic pressure under the same conditions.
The next system we consider is STA in water with three different kinds of added salt: NaCl, HCl, and LiCl. STA mol-ecules are spherical, more or less共see Fig.2in Ref.27兲, with
an effective diameter of 1.1 nm,28,29 so we set a = 0.55 nm. The structural formula for the polyanion SiW12O404−implies a molar mass MSTA= 2874.3 g mol−1. We assume that the pH is low enough for the molecule to be fully dissociated, i.e.,
Z = 4.
We determine the well parameters UA and␦ for the at-tractive interaction by fitting experimental data of the second virial coefficient in the same way as was done for lysozyme,7 except we now do not adjust Zeff. The second virial coeffi-cients for Li4STA, H4STA, and Na4STA are taken from Ref. 30and plotted in Fig.4. In each case, the added salt is XCl, where X represents the counterion of the crystal. The values of the dimensionless parameters = 1.80
= 0.645共Zeff/共1+兲兲2, Z, and Zeff pertaining to the data in Fig. 4 are given in Table II. We have set ␦= 0.05. A least squares fit to the data represented in Fig. 4 then gives UA = 3.30. In fact, there is a range of combinations of␦and UA that yield almost the identical curve as long as ␦exp UA ⬇1.36 and␦Ⰶ1, so our choice of␦= 0.05 is a bit arbitrary. This similarity with respect to the sole parameter␦exp UAis in accord with our approximation for B2 given by Eq.共5兲.
The solubilities for Li4STA, H4STA, and Na4STA have been measured by Zukoski et al.,30where the same electro-lytes are used as in the measurements of B2共see Table III兲.
The volume fraction of STA is given by
= SNAv0/ MX4STA, where S is the solubility of STA共note that here it is given in g/ml, whereas for lysozyme it was given in g/l兲, v0= 4a3/ 3 is the volume of a STA molecule and MX4STA is the molar mass, where X again represents the counterion in the respective cases. We have MH4STA = 2878.3 g mol−1, M
Li4STA= 2902.0 g mol−1, and MNa4STA = 2966.2 g mol−1. The stickiness parameter is determined FIG. 2. The dimensionless chemical potential of lysozyme in the fluid phase
as a function of the ionic strength at pH 4.0共diamonds兲, pH 4.5 共squares兲, and pH 5.4共triangles兲. See also TableI.
FIG. 3. The dimensionless pressure of lysozyme in the fluid phase as a function of the ionic strength at pH 4.0共diamonds兲, pH 4.5 共squares兲, and
pH 5.4共triangles兲. See also TableI.
FIG. 4. The second virial coefficient of STA as a function of the ionic strength. The second virial coefficient is scaled by the hard sphere value
B2HS. The experimental data are taken from Zukoski et al. 共Ref.30兲. The
added salt is LiCl共diamonds兲, HCl 共squares兲, and NaCl 共triangles兲, respec-tively, and in all cases the counterion of STA is the same as that of the salt. The solid line is a fit to the experimental data with UA= 3.30 and␦= 0.05.
TABLE II. Values of the bare charge Z of STA, the effective charge Zeff
关from Eq.共3兲兴 and the dimensionless interaction parameters= 1.80冑I and
= 0.645共Zeff/共1+兲兲2as a function of the ionic strength I. These entries
apply to the data plotted in Fig.4.
by the method described in Sec. II关see Eqs.共6兲–共13兲兴, using the values UA= 3.30 and␦= 0.05. The chemical potential and the osmotic pressure are again determined from Eqs. 共15兲 and共14兲, respectively共see TableIII兲. We display these
ther-modynamic variables as a function of the ionic strength in Figs.5and6.
IV. CRYSTAL MODEL: DONNAN EFFECT
Having computed the thermodynamic properties of the fluid phases of lysozyme and STA, and hence those of the respective crystal phases under the assumption of equilib-rium of the two phases, we now attempt to gain insight into them by introducing a simple model for the crystal. In the latter the spherical particles either touch or are very close. There are thus minute “surfaces of interaction” where the forces between two nearby spheres are predominantly attrac-tive. It is therefore reasonable to write the thermodynamic
potential ⍀ of a crystal of N spheres in a volume V as a superposition of attractive and electrostatic contributions to a first approximation,
⍀ =1 2k共c兲
共V − V0兲2
V0 + Nfel共c,Ic兲 + ⌸共S,I兲V −共S,I兲N.
共19兲 The crystal is immersed in a large reservoir at a constant osmotic pressure ⌸ and chemical potential containing a saturated solution of nanospheres at a solubility S and ionic strength I关⌸ andare given by Eqs.共14兲and共15兲, respec-tively兴. The crystal has elastic properties denoted by the modulus k which depends on the density c = N / V and the crystal would have a volume V0 in the absence of electro-static forces 共兩V−V0兩ⰆV0兲. Actually, the form of the elastic energy is more complicated and depends on the precise crys-tal habit31but the simple harmonic form in Eq.共19兲suffices for our purposes. There is a Donnan equilibrium共see below兲 TABLE III. The charge Z of STA, the effective charge Zeff关from Eq.共3兲兴, the dimensionless interaction parameter,and, the solubility S of X4STA, the
volume fraction, the dimensionless chemical potential共−0兲/kBT, and the dimensionless pressure⌸v0/ kBT as a function of the ionic strength I in the fluid
phase. Here the counterion is X+and the added salt is XCl.has been calculated using the effective charge Z eff. X I共M兲 Z Zeff S共g/ml兲 −0 kBT ⌸v0 kBT H 1.0 1.80 4.0 3.58 1.054 0.786 1.94 0.284 1.30 0.706 H 2.0 2.55 4.0 3.70 0.700 0.358 1.67 0.243 −0.48 0.375 H 3.0 3.13 4.0 3.76 0.536 0.255 1.36 0.198 −1.40 0.226 H 4.0 3.61 4.0 3.80 0.439 0.215 1.11 0.162 −1.91 0.158 H 5.0 4.03 4.0 3.83 0.373 0.193 0.57 0.0830 −2.65 0.077 Li 1.0 1.80 4.0 3.58 1.054 0.668 2.15 0.312 1.55 0.811 Li 2.0 2.55 4.0 3.70 0.700 0.352 1.85 0.267 −0.267 0.433 Li 3.0 3.13 4.0 3.76 0.536 0.255 1.36 0.197 −1.41 0.224 Li 4.0 3.61 4.0 3.80 0.439 0.215 0.81 0.118 −2.23 0.114 Li 5.0 4.03 4.0 3.83 0.373 0.193 0.32 0.0469 −3.16 0.045 Na 1.0 1.80 4.0 3.58 1.054 0.906 1.85 0.262 1.07 0.625 Na 2.0 2.55 4.0 3.70 0.700 0.359 1.67 0.236 −0.54 0.358 Na 3.0 3.13 4.0 3.76 0.536 0.255 1.36 0.192 −1.44 0.218 Na 4.0 3.61 4.0 3.80 0.439 0.215 0.74 0.104 −2.35 0.100 Na 5.0 4.03 4.0 3.83 0.373 0.193 0.46 0.0657 −2.86 0.062
FIG. 5. The dimensionless chemical potential of STA in the fluid phase as a function of the ionic strength. The added salt is LiCl 共diamonds兲, HCl 共squares兲, and NaCl 共triangles兲, respectively, and in all cases the counterion of STA is the same as that of the salt. See also TableIII.
which leads to a salt concentration Icwithin the interstitial region in the crystal. We adopt a continuum approximation: the electrostatic free energy N felis computed for a lattice of charged spheres embedded in a solvent of uniform permittiv-ity⑀and electrolyte concentration Ic.
At equilibrium, ⍀ must be minimized 共⍀/V = 0;
⍀/N = 0兲 so that ⌸ ⯝ ⌸el− k
冉V − V0 V0
冊+1 2c dk dc
冉V − V0 V0
冊2 , 共20兲 ⯝el+ 1 2 dk dc
冉V − V0 V0
冊2 . 共21兲
We have introduced the electrostatic counterparts of the os-motic pressure and the chemical potential of a charged sphere in the crystal phase on the right hand sides of Eqs.
共20兲and共21兲. In Eq. 共20兲the elastic term proportional to k may easily be of order⌸el but the quadratic form is negli-gible. In view of the fact that ⌸el= O共cel兲, we then have ⯝elto a good approximation from Eq.共21兲. In effect, as we change the ionic strength of the fluid phase, the solubility
S and the salt concentration Ic within the crystal readjust themselves whereas the volume V remains virtually constant. The chemical potential is modified only by virtue of the change in electrostatic shielding about a sphere in the lattice. But a substantial hydrostatic pressure may be exerted within the crystal as we decrease its volume a bit.
Next, we compute the electrostatic properties of the crystal. The colligative properties of salt-free polyelectro-lytes are often addressed in terms of a cell model in which a test cylinder is surrounded by a boundary of similar symme-try on which the electric field vanishes.32 The boundary ef-fectively replaces the effect of the surrounding particles on the test particle. This picture is reasonable at low volume fractions but must break down at high concentrations when the electric field is highly heterogeneous. In the latter case, one of us has advocated focusing on the voidlike regions instead of on a test particle共see Ref.33which deals with a hexagonal lattice of DNA at very high concentrations兲. Thus, in a crystal of spheres we may distinguish very small regions between particles that almost touch which we view as thin boundary layers, and larger voids which we will simply ap-proximate by spheres.共We are here concerned with spheres of high charge density which leads to counterions being “condensed.” At low charge densities, it is possible to give a more general analysis; see Appendix B兲. Discrete charge ef-fects should prevail when evaluating the electrostatics of the boundary layers. These energies are here assumed to be in-dependent of the ionic strength since the relevant scales in the boundary layers are very small in crystals of nanopar-ticles.
We therefore first solve the Poisson-Boltzmann equation for a charged void or spherical cavity of radius b without salt and then discuss the effect of monovalent salt via a Donnan equilibrium. The charge density on the surface of the cavity is uniform and the total number of charges is Z. In view of electroneutrality there are Z counterions in the cavity, each bearing charge −q. Within a mean-field analysis, the
counter-ion density 共r兲 inside the cavity is given by a Boltzmann distribution in terms of the electrostatic potential ⌿共r兲 at a distance r from its center,
共r兲 =¯e q⌿/kBT. 共22兲
We choose⌿=0 at the center of the cavity so that¯ is the
actual charge density there. The charge density −q is also related to ⌿ by Poisson’s equation,
⑀ , 共23兲
leading to the Poisson-Boltzmann equation32which we con-veniently express in the scaled form
⬘共x兲 = e
Here, we have defined −2⬅4Q¯, x ⬅r/, and
⬅q⌿/kBT, where may be interpreted as a screening length. The two additional boundary conditions are
⬘共0兲 = 0 共25兲
owing to symmetry, and
冊=⌳ ⬅ QZ b 共26兲
signifying the relation between the electric field and the charge density at the surface of the cavity.
For small x, Eq. 共24兲 admits a series expansion 共x兲 = Ax2+ Bx4+¯ with A=1/6 and B=O共1兲 independent of the value of the dimensionless variable ⌳. As ⌳ tends to zero, Eq. 共26兲 reduces to the condition of electroneutrality. Elec-trostatic screening vanishes in this limit and there are no counterions “condensed” on the surface of the sphere. It is straightforward to solve Eq. 共24兲 numerically starting with 共x兲→1
6x2 as x→0. We have fitted the solution to the con-venient approximation, 共x兲 ⬇ − 2 ln
冉1 − x 2 12− x4 1440− x6 45 330.3
which is accurate to within 0.6% for 0艋x艋3.273 687 关共x兲 diverges at x⬇3.273 687 34兴. This leads to an effective charge given by Zeff⬅4b 3¯ 3 = Z 3⌳
冊2 . 共28兲
This is always less than the actual charge Z which one may interpret as a certain fraction of counterions being associated near the surface if⌳⬎0. The effective charge Zefftends to Z as ⌳→0 共for a general analysis of this limit, see Appendix B兲.
repre-sent effectively the potential of mean force between the par-ticles. In the case of excess salt, we then use the McMillan-Mayer theory to calculate the statistical mechanical properties of the fluid as has been done in Sec. II 关see Eq.
共2兲; this line of argumentation goes back to Stigter34兴. The situation is decidedly different when the particles are posi-tionally ordered as in a crystal. The double layers are forced to overlap in that case. A usual 共Donnan兲 approximation is then to suppose those points at zero electric field are in equi-librium with the reservoir.32 For the cavities in the crystal, this yields
Ic共¯ + Ic兲 = I2 共29兲 in view of the equality of the chemical potentials of the small ions in the respective phases. The osmotic pressure is given by the additivity rule as argued by Oosawa for polyions within conventional cell models,32
⌸ = 共¯ + 2Ic− 2I兲kBT =¯k BT关
冑1 + w2− w兴, 共30兲 w⬅2I
The ions have been considered as ideal and the electrostatic stress is zero in Eq. 共20兲. The chemical potential of the charged cavity, accurate to the same level of approximation, is readily computed from Eq.共30兲共this is analogous to simi-lar calculations for cell models of long charged rods35 兲,
=ref+ ZeffkBT 2 ln
冑1 + w2+ 1
冑1 + w2− 1
whererefis a reference chemical potential independent of the concentration of salt, and not identical with0of Sec. II. Because the number of particles in the crystal is equal to the number of cavities, Eq. 共31兲 also represents the chemical potential of a charged sphere carrying Z charges but with a differentref.
A. Comparison with experiment 1. Lysozyme crystal
The volume per lysozyme molecule in the tetragonal crystal is 29.6 nm3 共see Sec. III B兲. The radius of the effec-tive sphere is 1.60 nm so the volume of a cavity is 12.4 nm3 and b = 1.43 nm. In Table IV, we show values of Z as a function of the ionic strength I at three values of the pH. From these we calculate the dimensionless quantities⌳, b/, and Zeffvia the Poisson-Boltzmann equation. Then the pres-sure and the chemical potential are evaluated using Eqs.共30兲 and共31兲 共see TableIV兲. The curves in Fig.7 represent the chemical potential computed in this manner together with the predictions from the theory of the liquid state as displayed in Fig.2. The former have been shifted by an amount which is unknown in the present theory.
TABLE IV. The ionic strength I, the actual number of charges Z, the effective number Zeffthe chemical potential, and the osmotic pressure⌸ for a lysozyme
crystal共the reference chemical potential has been set equal to zero兲.
pH I共% w/v兲 I共M兲 Z ⌳ b / Zeff w kBT ⌸v0 kBT 4.0 2.0 0.40 11.1 5.51 2.52 4.27 1.41 2.83 1.92 4.0 3.0 0.57 11.2 5.56 2.53 4.29 2.00 2.07 1.43 4.0 4.0 0.74 11.4 5.66 2.54 4.32 2.57 1.64 1.14 4.0 5.0 0.92 11.6 5.76 2.55 4.35 3.14 1.36 0.95 4.0 7.0 1.26 11.7 5.81 2.55 4.37 4.30 1.01 0.71 4.5 2.0 0.40 10.2 5.06 2.48 4.13 1.45 2.66 1.81 4.5 3.0 0.57 10.3 5.11 2.49 4.15 2.06 1.94 1.34 4.5 4.0 0.74 10.3 5.11 2.49 4.15 2.68 1.52 1.06 4.5 5.0 0.92 10.4 5.16 2.49 4.17 3.28 1.25 0.88 4.5 7.0 1.26 10.4 5.16 2.49 4.17 4.51 0.92 0.64 5.4 2.0 0.40 9.1 4.52 2.42 3.94 1.53 2.42 1.66 5.4 3.0 0.57 9.1 4.52 2.42 3.94 2.18 1.75 1.21 5.4 4.0 0.74 9.2 4.57 2.43 3.95 2.81 1.38 0.96 5.4 5.0 0.92 9.2 4.57 2.43 3.95 3.46 1.13 0.79 5.4 7.0 1.26 9.1 4.52 2.42 3.94 4.77 0.82 0.58
FIG. 7. The chemical potential of lysozyme in the fluid phase as a function of the ionic strength at pH 4.0共diamonds兲, pH 4.5 共squares兲, and pH 5.4 共triangles兲 共see Fig.2兲. The solid lines denote predictions from the theory of
the crystalline state关Eq.共31兲兴, with the effective charge from TableIV. The shift in chemical potential in units of kBT has been chosen to be 7.4共light
gray line, pH 4.0兲, 7.3 共black line, pH 4.5兲, and 7.15 共dark gray line, pH 5.4兲, respectively. The dashed line denotes the theory of the crystal for
2. STA crystals
In order to compute the chemical potential we first need to discuss the crystal habits of STA. It is known that H4STA is fully dissociated for a pH larger than 5.36 Zukoski and co-workers.5,30,37 failed to mention the pH at which their measurements were performed, though they did deduce that all forms of STA are dissociated in their experiments judging from the conductivities of their solutions.
a. H4STA· 31H2O. This crystallizes at room temperature38 in the tetragonal form 共long axis=1.856 nm, short axes= 1.301 nm;39 there are two STA molecules per unit cell of 3.142 nm3兲. We have earlier set the radius of an STA ion equal to 0.55 nm共see Sec. III C兲 so the volume of H2O per STA molecule is 0.874 nm3 or b = 0.593 nm. In Refs. 5 and37 the water content of this crystal is given in terms of the molecular formula H4STA· 31H2O.
b. Li4STA· 24H2O / Li4STA· 26H2O. Kraus described two forms of Li4STA with 24 H2O and 26 H2O molecules attached, respectively.40 Both crystals are rhombohedral 关short axes in both cases=1.559 nm, long axis=3.898 nm in the former, long axis= 4.118 nm in the latter; the angle be-tween the short axes= 120°共Ref.39兲兴. Kraus also mentioned
that one Li ion should probably be replaced by one H ion. There are actually three different numbers quoted for the water content of Li4STA· nH2O in Refs. 5, 30, and 37: n = 21, 24, and 26! We have opted for n = 25, namely, the av-erage number for the crystal habits generally accepted. As there are six STA molecules per unit cell, the volume of crystal per STA molecule is 1.406 nm3and the radius of our effective cavity is b = 0.553 nm.
c. Na4STA· 18H2O. This crystallizes in the triclinic form within a narrow range around 308 K.38The absolute dimen-sions of the unit cell do not seem to be known. We thus estimate the amount of H2O per STA molecule via the mo-lecular formulas. The water content in Na4STA· nH2O is stated to be n = 18 in Ref.37and n = 14 in Ref.5. The latter value seems too low and is possibly a misprint since n should be equal to 20 according to the usual citation.41Accordingly, we adopt n = 18 here to be used in the solubility studies.30A
molecule of H2O has a volume of 0.0285 nm3which is based on the amount of H2O in the unit cells of H4STA· 31H2O and Li4STA· 26H2O. Therefore, Na4STA· 18H2O has 0.513 nm3H2O per STA molecule so we have b = 0.496 nm. Overall, it is not clear how much H2O is exactly present in the STA crystals. Fortunately, the chemical potential关Eq.
共31兲兴 depends only logarithmically on this quantity so the data compiled in Table Vare not so sensitive to this type of uncertainty. The predicted chemical potentials are depicted as curves in Fig.8 together with the computations from our theory of the liquid state共Fig.5兲.
Except for a slight downward adjustment of the effective charge of lysozyme in the fluid phase, there are essentially no adjustable parameters in our analysis. The adjustment is TABLE V. Same as TableIVbut now for X4STA· nH2O. Here n = 31 when X = H, n = 25 when X = Li and n = 18 when X = Na.
X I共% w/v兲 I共M兲 Z ⌳ b / Zeff w kBT ⌸v0 kBT H 1.0 0.60 4.0 4.789 2.452 1.67 0.629 2.08 0.738 H 2.0 1.20 4.0 4.789 2.452 1.67 1.257 1.22 0.466 H 3.0 1.81 4.0 4.789 2.452 1.67 1.886 0.85 0.332 H 4.0 2.41 4.0 4.789 2.452 1.67 2.514 0.65 0.256 H 5.0 3.01 4.0 4.789 2.452 1.67 3.143 0.52 0.207 Li 1.0 0.60 4.0 5.134 2.488 1.61 0.531 2.23 0.950 Li 2.0 1.20 4.0 5.134 2.488 1.61 1.062 1.35 0.626 Li 3.0 1.81 4.0 5.134 2.488 1.61 1.594 0.95 0.455 Li 4.0 2.41 4.0 5.134 2.488 1.61 2.125 0.73 0.353 Li 5.0 3.01 4.0 5.134 2.488 1.61 2.656 0.59 0.288 Na 1.0 0.60 4.0 5.721 2.542 1.51 0.410 2.45 1.374 Na 2.0 1.20 4.0 5.721 2.542 1.51 0.819 1.55 0.970 Na 3.0 1.81 4.0 5.721 2.542 1.51 1.229 1.12 0.728 Na 4.0 2.41 4.0 5.721 2.542 1.51 1.639 0.87 0.575 Na 5.0 3.01 4.0 5.721 2.542 1.51 2.049 0.71 0.473
FIG. 8. Chemical potential of STA in the fluid phase as a function of the ionic strength共see Fig.5兲. Salt added: LiCl 共diamonds兲, HCl 共squares兲, and
NaCl共triangles兲 共counterion of STA is the same as that of the salt兲. The solid lines denote predictions from the theory of the crystalline state关Eq.共31兲兴, with the effective charge from TableV. The shift in chemical potential in units of kBT is 2.3 共black line, H4STA· 31H2O兲 2.4 共 dark gray line,
Li4STA· 25H2O兲, and 2.55 共light gray line, Na4STA· 18H2O兲, respectively. The dashed line denotes predictions from the theory of the crystal for Zeff
by one unit only which is insignificant compared with the approximations inherent in the standard electrostatic theory. The adhesion parameters are completely constrained by the second virial curves 共Figs. 1 and 4兲. We predict that the
chemical potentials in the fluid and solid phases should co-incide apart from an unimportant shift in the vertical offset because the reference potential is not known exactly for the crystal. This appears to be almost the case for lysozyme共see Fig.7兲 but there is an appreciable disparity between the
re-spective curves in the case of the silicotungstates共see Fig.8兲.
Nevertheless, we note that the shapes of the curves are the same which implies that the logarithmic form in Eq. 共31兲 appears to be confirmed, i.e., the Donnan effect seems to apply to crystals of charged nanoparticles. This is borne out by adjusting Zeffupward somewhat for both types of crystals. We then actually attain coincident curves共see Figs.7and8兲.
A further implication is that the precise crystal structure is unimportant with regard to the ionic-strength dependence of . Equation 共31兲 results from approximating the cavities within the crystals by spheres; the detailed electrostatics is independent of the salt concentration.
The coexistence equation for the osmotic pressure yields little information 关see Eq. 共20兲兴 because it is unclear at present how to relate the adhesive forces between spheres to the elastic properties of the crystal. To compute the latter we need insight in the forces between the particles at the ang-strom level which we do not have at present. Adhesive inter-actions appear to play a minor role in the STA crystals for the fluid and crystal pressures are quite close共compare TableIII
andV兲. By contrast, in lysozyme crystals the osmotic
pres-sure due to electrostatic forces is largely balanced by sticky interactions between touching protein molecules. In a similar vein there is a marked difference between the two colloids with regard to their respective ionic strengths under theta conditions when B2 equals zero 共see Figs.1 and 4兲. These salt concentrations may be estimated with the help of Eq.共5兲. Although ␦exp UA= 1.36 for STA is not substantially less than the respective value 3.33 for lysozyme, the concentra-tions differ appreciably because of the exponential screening term multiplying the attraction in Eq.共5兲.
It is wise to emphasize the shortcomings in the approxi-mations introduced in the electrostatic interactions. Discrete charge effects have been disregarded entirely. At the same level of approximation we have not addressed the electrostat-ics of the minutely thin boundary layers between almost touching spheres within the crystal phase. There are cavities at nanometer scales and these are assumed to give rise to the ionic-strength dependence of the free energy of the crystal. The Donnan approximation used suffers from the same drawback as always: the effective charge Zeffis posited to be independent of the electrolyte in the crystal and thus the reservoir共the fluid phase in our case兲. It would be interesting to study the fluid-crystal coexistence of globular particles of low charge density. The counterions in the crystal would then be essentially free共see Appendix B兲 and there would be less uncertainty about the magnitude of the electrostatic interac-tions.
There is another potential problem in the fluid phases of silicotungstates. At 1M electrolyte, the solubilities of STA
are remarkably high共see TableIII兲. It would appear that the
counterions arising from STA should contribute to the screening on a par with the salt ions. This is not borne out by the present analysis, however, since there is no leveling off of the chemical potentials in the crystal phases in Figs.7and
8. Nevertheless, a liquid state theory of concentrated charged nanoparticles needs to be developed in which the counterions are duly accounted for. We note that the interaction between the particles is not pairwise additive in that case.
In summary, we have provided a semiquantitative expla-nation for the ionic-strength dependence of the fluid-crystal coexistence of suspensions of charged nanoparticles. We be-lieve this explanation is especially forceful because we have considered two rather disparate types of globular particles in detail. In particular, the solubility curves of lysozyme and silicotungstate differ markedly, yet the curves for the chemi-cal potentials turn out to have the same form.
The authors thank Professor E. Trizac for correspon-dence on the Poisson-Boltzmann equation.
APPENDIX A: PHASE DIAGRAM OF HARD SPHERES INTERACTING BY ATTRACTIVE YUKAWA
ity variable for the fluid phase,8it has nothing to do with the statistical properties of the crystal in which the configura-tions are weighted totally differently than those in the fluid.
APPENDIX B: POISSON-BOLTZMANN EQUATION IN A CRYSTAL OR POROUS MEDIUM
Here, we present only a sketch of a general analysis of the Poisson-Boltzmann equation for the electrostatic poten-tial ⌿共r兲 at position r within the aqueous interstitial space inside a crystal 共which may be considered to be a porous medium兲, under appropriate conditions. The particles in the crystal are positively charged and simple salt is absent at first. The potential is again related to the counterion density 共r兲 via the Poisson equation 共23兲. Now it is possible to discern some point P in the void between several particles where the potential is a local minimum and where the den-sity is¯P共0兲 共see Fig.10兲. Point P is chosen as the origin.
If the potential is scaled analogously as in Sec. IV, we have 共r兲=¯Pexp共r兲 关see Eq. 共22兲兴. Thus, the Poisson-Boltzmann equation may be written as
where the screening lengthPis given byP
−2= 4Q¯ P. In general, it is difficult to address 共B1兲 because P is unknown. But it is possible to progress if we suppose 兩d兩 ⱗPwhere兩d兩 is the largest vector distance between P and a point on the surface of the surrounding spheres 共i.e., those belonging to a cluster enclosing the void centered on P兲. An inner solution of共B1兲must have the formin共r/P兲 and may be written as a Taylor expansion to second order,
in共r兲 = 1 2rr:
冏2 in rr
if兩d兩ⱗP. There is an outer solutionoutneeded to accom-modate for the complicated boundaries. Then, we have a boundary condition on the electric field at r = d in terms of outwhich we rewrite in terms ofin
冏r=0= 4k1bQ. 共B3兲 Here,bis the uniform density of charge on a sphere and k1 is a numerical coefficient of order unity associated with the matching of the inner and outer solutions. The effect of an internal permittivity is disregarded. The left-hand side of
共B3兲 scales as P −2
implying that¯P must be proportional to b. In view of electroneutrality we also require the average of 共r兲 to be proportional to b. Hence, the potential共r兲 must be very small, which is consistent with the initial
An-satz 共B2兲. We conclude that for small enough cavitylike voids, the density of counterions is approximately constant so that the effective charge density is virtually equal to the actual charge density. In that case, when the crystal is im-mersed in a reservoir containing monovalent electrolyte, Eqs.
共30兲 and共31兲are valid with¯ simply given by the concen-
tration of counterions in the interstitial space between the spheres; Zeff= Z in Eq. 共31兲. Because 兩d兩=O共a兲, we ulti-mately require ZQ / aⰆ1 as a necessary and sufficient condi-tion for this to hold true. In the spherical cavity approxima-tion introduced in Sec. IV, we have b = O共a兲 so ⌳Ⰶ1 is effectively the same requirement共which led to Zeff= Z兲.
1A. George and W. W. Wilson, Acta Crystallogr., Sect. D: Biol.
Crystallogr. D50, 361共1994兲.
2A. George, Y. Chiang, B. Guo, A. Arabshahi, Z. Cai, and W.W. Wilson,
Methods Enzymol. 276, 100共1997兲.
3B. Guo, S. Kao, H. McDonald, A. Asanov, L.L. Combs, and W.W.
Wil-son, J. Cryst. Growth 196, 424共1999兲.
4C. Haas, J. Drenth, and W.W. Wilson, J. Phys. Chem. B 103, 2808
5D. Rosenbaum, P.C. Zamora, and C.F. Zukoski, Phys. Rev. Lett. 76, 150
6D. F. Rosenbaum and C.F. Zukoski, J. Cryst. Growth 169, 752共1996兲. 7P. Prinsen and T. Odijk, J. Chem. Phys. 121, 6525共2004兲.
8P. Prinsen, J.C. Pàmies, T. Odijk, and D. Frenkel, J. Chem. Phys.共to be
published兲, e-print cond-mat/0603716.
9C. Haas and J. Drenth, J. Phys. Chem. B 102, 4226共1998兲. 10C. Haas and J. Drenth, J. Cryst. Growth 196, 388共1999兲.
11R. A. Curtis, H.W. Blanch, and J.M. Prausnitz, J. Phys. Chem. B 105,
12E. Cacioppo and M.L. Pusey, J. Cryst. Growth 114, 286共1991兲. 13M. Boström, D.R. M. Williams, and B.W. Ninham, Langmuir 17, 4475
14F. W. Tavares, D. Bratko, H.W. Blanch, and J.M. Prausnitz, J. Phys.
Chem. B 108, 9228共2004兲.
15M. Aubouy, E. Trizac, and L. Bocquet, J. Phys. A 36, 5835共2003兲. 16R. Fowler and E.A. Guggenheim, Statistical Thermodynamics
共Cam-bridge University Press, Cam共Cam-bridge, 1956兲.
17W. C. K. Poon, S.U. Egelhaaf, P.A. Beales, A. Salonen, and L. Sawyer, J.
Phys.: Condens. Matter 12, L569共2000兲; P.B. Warren, ibid. 14, 7617 共2002兲.
18R. J. Baxter, J. Chem. Phys. 49, 2770共1968兲.
19H. C. Andersen, J.D. Weeks, and D. Chandler, Phys. Rev. A 4, 1597
20J. P. Hansen and I.R. McDonald, Theory of Simple Liquids共Academic,
21B. Barboy, J. Chem. Phys. 61, 3194共1974兲. 22L. K. Steinrauf, Acta Crystallogr. 12, 77共1959兲.
23A. Nadarajah and M.L. Pusey, Acta Crystallogr., Sect. D: Biol.
Crystallogr. 52, 983共1996兲.
24V. Mikol, E. Hirsch, and R. Giegé, J. Mol. Biol. 213, 187共1990兲. 25D. E. Kuehner, J. Engmann, F. Fergg, M. Wernick, H. W. Blanch, and J.
M. Prausnitz, J. Phys. Chem. B 103, 1368共1999兲.
26M. Riès-Kautt, A. Ducruix, and A. van Dorsselaer, Acta Crystallogr.,
Sect. D: Biol. Crystallogr. 50, 366共1994兲.
27M. Ge, A. A. Gewirth, W. G. Klemperer, and C. G. Wall, Pure Appl.
Chem. 69, 2175共1997兲.
28M. C. Baker, P. A. Lyons, and S. J. Singer, J. Am. Chem. Soc. 77, 2011
29T. Kurucsev, A. M. Sargeson, and B. O. West, J. Phys. Chem. 61, 1567
30C. F. Zukoski, D. F. Rosenbaum, and P. C. Zamora, Chem. Eng. Res. Des. 74, 723共1996兲.
31L. D. Landau and E. M. Lifshitz, Theory of Elasticity, 3rd ed.共Pergamon,
32F. Oosawa, Polyelectrolytes共Dekker, New York, 1971兲.
33T. Odijk, Philos. Trans. R. Soc. London, Ser. A 362, 1497共2004兲. 34D. Stigter, Biopolymers 16, 1435共1977兲.
35T. Odijk and F. Slok, J. Phys. Chem. B 107, 8074共2003兲.
36M. J. Kronman and S. N. Timasheff, J. Phys. Chem. 63, 629共1959兲. 37P. C. Zamora and C. F. Zukoski, Langmuir 12, 3541共1996兲. 38G. Wyrouboff, Z. Kristallogr. 29, 659共1898兲.
39H. T. Evans, in Perspectives in Structural Chemistry, edited by J. D.
Dunitz and J. A. Ibers共Wiley, New York, 1971兲, Vol. IV, pp. 8–21.
40O. Kraus, Z. Kristallogr. 94, 256共1936兲.
41R. J. Meyer, Gmelins Handbuch der Anorganischen Chemie, Wolfram,
共Verlag Chemie, Berlin, 1933兲.
42M. Dijkstra, Phys. Rev. E 66, 021402共2002兲.